tunable cu enrichment enables designer syngas ... tunable cu enrichment enables designer syngas...
Post on 28-Jun-2020
Embed Size (px)
Tunable Cu Enrichment Enables Designer Syngas Electrosynthesis from CO2 Michael B. Ross,†,‡ Cao Thang Dinh,‡,§ Yifan Li,†,∥ Dohyung Kim,⊥ Phil De Luna,‡,#
Edward H. Sargent,*,‡,§ and Peidong Yang*,†,‡,∥,⊥,¶,□
†Department of Chemistry, ⊥Department of Materials Science and Engineering, and □Kavli Energy Nanosciences Institute, University of California, Berkeley, Berkeley, California 94720, United States ‡Bio-Inspired Solar Energy Program, Canadian Institute for Advanced Research, Toronto, Ontario M5G 1Z8, Canada §Department of Electrical and Computer Engineering, University of Toronto, Toronto, Ontario M5S 3G4, Canada ∥Chemical Sciences Division and ¶Materials Sciences Division, Lawrence Berkeley National Laboratory, Berkeley, California 94720, United States #Department of Materials Science and Engineering, University of Toronto, Toronto, Ontario M5S 3E4, Canada
*S Supporting Information
ABSTRACT: Using renewable energy to recycle CO2 provides an opportunity to both reduce net CO2 emissions and synthesize fuels and chemical feedstocks. It is of central importance to design electro- catalysts that both are efficient and can access a tunable spectrum of products. Syngas, a mixture of carbon monoxide (CO) and hydrogen (H2), is an important chemical precursor that can be converted downstream into small molecules or larger hydrocarbons by fermentation or thermochemistry. Many processes that utilize syngas require different syngas compositions: we therefore pursued the rational design of a family of electrocatalysts that can be programmed to synthesize different designer syngas ratios. We utilize in situ surface- enhanced Raman spectroscopy and first-principles density functional theory calculations to develop a systematic picture of CO* binding on Cu-enriched Au surface model systems. Insights from these model systems are then translated to nanostructured electrocatalysts, whereby controlled Cu enrichment enables tunable syngas production while maintaining current densities greater than 20 mA/cm2.
■ INTRODUCTION Relentless improvements in renewable energy generation provide new opportunities for storing and harnessing electrical energy. In particular, increasingly abundant and inexpensive sources of electrons provide synthetic opportunities to replace conventional chemical processes with renewable powered ones.1−5 In addition to mild reaction conditions, these renewable powered electrochemical reactions could enable decreased production costs relative to conventional approaches, particularly for the production of feedstock chemicals from CO2.
2,6 However, CO2 reduction reaction (CO2RR) electro- catalysts have several remaining fundamental and performance- related challenges, particularly related to low production rates, limited product versatility, and poor energy efficiencies.6,7
Although direct electrosynthesis of multicarbon products remains elusive, catalytic efficiencies and production rates for single-carbon products, such as CO and formic acid, provide more immediate opportunities for electrochemical CO2 valor- ization. Synthesis gas (syngas) made using renewable powered CO2RR is particularly attractive because it can subsequently be upgraded to longer hydrocarbons by Fischer−Tropsch chemistry, syngas fermentation, and individual small-molecule
synthesis.2,4,5,8,9 Desirably, the syngas electrosynthesis catalyst will operate at room temperature, in a single reactor, and with high efficiency and production rates. These attributes, combined with the ability to tailor the composition of syngas for each downstream process (such as 0.6 H2:CO for Fischer− Tropsch reactors, 2 H2:CO for methanol synthesis, and 0.3−1 H2:CO for syngas fermentation),
4,5,8,9 would provide a flexible platform for integration with existing chemical infrastructure. Several electrocatalytic systems provide either rapid reaction turnovers or a variety of syngas compositions; however, there exist no prior reports of a single electrocatalyst that exhibits high production rates (at low overpotential) combined with systematic and wide-ranging syngas composition control.10−15
Herein, we report a strategy where the composition of syngas produced by a nanostructured Au electrocatalyst can be finely controlled using Cu underpotential deposition while maintain- ing high geometric current densities (production rates) at low overpotentials for CO2RR (Figure 1a). Within this scope, underpotential deposition provides a quantitative and system-
Received: May 12, 2017
© XXXX American Chemical Society A DOI: 10.1021/jacs.7b04892 J. Am. Chem. Soc. XXXX, XXX, XXX−XXX
atic means by which the ratio of Au and Cu atoms at the surface can be tuned. Such control changes the electronic structure at the catalyst surface,7,16,17 which we hypothesized would influence CO binding and thereby provide a method for tuning the relative selectivity of CO electrosynthesis and the hydrogen evolution reaction (HER).18,19 In situ surface- enhanced Raman spectroscopy (SERS) is used to interrogate changes in the coordination and binding characteristics of adsorbed CO (CO*) on model Au SERS substrates. In turn, fundamental insights from both in situ SERS and density functional theory (DFT) calculations are translated from model systems to nanostructured electrocatalysts that provide high electrochemical activity (>20 mA/cm2) for the most industri- ally relevant syngas compositions.
■ RESULTS AND DISCUSSION Design of Cu-Enriched Model Electrocatalysts. We
focus on structures in which Au surface atoms are replaced with Cu atoms in ordered monolayers; this serves as an approximation of surfaces that are increasingly Cu-enriched (Figure 1b). Indeed, the calculated projected density of states, which describes the electronic states at the surface, shows each Cu-enriched slab has distinct electronic properties. Importantly, these differences are most pronounced in the d-band electrons that dominate molecular adsorption, suggesting that Cu- enriched slabs should exhibit catalytic activity distinct from pure Au and Cu or their alloys.18−20 To realize such architectures, electrochemical underpotential deposition (UPD) was used to control the extent of Cu enrichment (Figure 2a). UPD occurs when the electrochemical deposition of a less noble species onto a more noble metal is thermodynamically favorable, but the deposition of the less noble species onto itself in unfavorable. This enables precise control over metal deposition because UPD is self-terminating at a single monolayer.21 Additionally, the use of Au as a substrate provides a platform where the binding of CO* can be monitored in situ with SERS, a nondestructive technique where the Raman scattering of surface-adsorbed molecules can be enhanced by 105−1010.22 By combining the precision of UPD with the sensitivity of SERS, one can manipulate the electronic and geometric properties of the catalyst surface (Figure 1b), by virtue of changing the extent of Cu enrichment, while monitoring changes in CO*.
Synthesis and Characterization of Au Architectures Enriched by Cu Underpotential Deposition. Cu-enriched Au electrodes were synthesized by electrochemical roughening, which renders them SERS-active, followed by Cu UPD (Figure 2b, S1, Methods), where stable cyclic voltammetry (CV) traces are indicative of Cu (sub)-monolayer deposition. Throughout this work three potential windows were used that correspond to approximately 1/3 monolayer CuUPD (Θ = 1/3), 2/3
Figure 1. Cu enrichment of Au surfaces enables tuning the composition of electrosynthesized syngas. (a) Scheme depicting the relationship between Cu-enriched Au surface, in situ characterization of CO* coordination, and syngas composition. (b) Calculated d-band electronic states for increasingly Cu-enriched Au surfaces.
Figure 2. Sub-monolayer Cu underpotential deposition on Au SERS- active model electrodes. (a) Scheme of Cu underpotential deposition. (b) Cyclic voltammograms for increasingly wide Cu underpotential deposition windows (no Cu, yellow; 1/3 of the window, orange; 2/3 blue; and 3/3 purple). (c) Scanning electron micrographs of a roughened Au SERS-active electrode before (top, yellow box) and after (bottom, purple box) deposition of Cu using the full (3/3) underpotential deposition window; scale bars are 100 nm. (d) Representative Au (top) and Cu (bottom) X-ray photoelectron spectra (here from the 3/3 window Cu underpotential deposition).
Journal of the American Chemical Society Article
DOI: 10.1021/jacs.7b04892 J. Am. Chem. Soc. XXXX, XXX, XXX−XXX
monolayer CuUPD (Θ = 2/3), and one full monolayer CuUPD (Θ = 1). Although previous literature has shown that ordered Cu monolayers can form on single-crystalline Au surfaces, the broad features in the voltammograms indicate that Cu is deposited onto a variety of coordination environments on the polycrystalline Au surface.21,23
Further characterization indicates that the extent of Cu enrichment is indeed controlled while the electrode morphol- ogy is maintained after UPD. Scanning electron microscopy (SEM) does not indicate restructuring of the SERS-active nanoscale features (Figure 2c), while X-ray photoelectron spectroscopy (XPS) confirms that wider UPD windows increase the ratio of Cu to Au atoms at the surface (Figure 2d, Table S1). Additionally, SER spectra of the Au substrate before and after UPD indicate the displacement of adsorbed chloride remaining after the roughening procedure without showing any ne